INTERNATIONAL JOURNAL FOR NUMERICAL METHODS IN ENGINEERING, VOL. 39, 1405- 1417 (1996) A FAST NUMERICAL METHOD FOR ISOTHERMAL RESIN TRANSFER MOLD FILLING R. S. MAIER Minnesota Supercomputer Center, Inc., and Army High Performance Computing Research Center, I100 Washington Avenue So., Minneapolis, M N 55415 U.S.A. T. F. ROHALY Army Research Laboratory, Aberdeen Proving Grounds, MD, US.A. S. G. ADVANI Department of Mechanical Engineering, University of Delaware, Newark, DE, U.S.A. K. D. FICKIE Army Research Laboratory, Aberdeen Proving Grounds, M D 21005, U.S.A. SUMMARY An efficient numerical scheme is presented for simulating isothermal flow in resin transfer molding. The problem involves transient, free surface flow of an incompressible fluid into a non-deforming porous medium. A new variant of the Control Volume Finite Element (CVFE) algorithm is explained in detail. It is shown how the pressure solutions at each time step can be obtained by adding a single row and column to the Cholesky factorization of the stiffness matrix derived from a finite element formulation for the pressure field. This approach reduces the computation of a new pressure solution at each time step to essentiallyjust two sparse matrix back-substitutions.The resulting performance improvement facilitates interactive simulation and the solution of inverse problems which require many simulations of the filling problem. The computational complexity of the calculation is bounded by O(n2’’),where n is the number of nodes in the finite element mesh. A 100-fold speedup over a conventional CVFE implementation was obtained for a 2213-node problem. KEY WORDS RTM;control volume; free surface; porous medium; sparse matrix RESIN TRANSFER MOLD FILLING PROBLEM Resin Transfer Molding (RTM) is an emerging manufacturing technology well-suited for fabricating large structural components made of composite materials. Since the process involves matched metal tooling, the technique seems ideal for situations requiring close tolerances. Construction of aircraft structures and vehicle components fit this characterization. Furthermore, liquid injection molding represents one of the most economical means of manufacturing. RTM is an adaptation on a process widely used for plastics. Instead of injecting into an empty cavity, the mold is packed with a woven fibre preform. The RTM process has two main stages: filling the mold with a resin/catalyst mixture and curing the part. At present, most of the difficulties of incorporating RTM revolve around the filling. To create an acceptable composite part requires the preform to be completely impregnated with resin. This CCC 0029-5981/96/081405- 13 0 1996 by John Wiley & Sons, Ltd. Received 24 May I994 Revised 28 April 199.5 1406 R. S. MAIER ET AL. is largely controlled by the fluid dynamics of the resin flow into the fibre reinforcement. The conditions which most strongly influence the flow are mold geometry, resin rheology, preform permeability, and location of the injectors and vents. The first three are typically determined by the part design itself; the last one is a manufacturing consideration. Incorrect placement of the injectors and vents for a given geometry and resin/preform system will create dry spots in the cured part. To enhance the economic viability of RTM applications, it is desirable to evaluate mold design prior to mold construction, via computer-based methods. Predictive modelling of resin flow through a fibre preform is currently an important priority in mold design and evaluation, because of the need to predict fill times and wet-out patterns. Ongoing research also includes control algorithms for the filling stage, using networks of embedded sensors and a fast filling simulation.'*2 Simulation of the RTM process may be isothermal or non-isothermal, depending upon whether temperature effects are accounted for in the model. During filling, resin viscosity is affected by temperature variations. During curing, gel times are affected by temperature profiles. For a mathematical formulation of the non-isothermal RTM process, see Reference 3. We focus on the isothermal case under the assumption of minimal temperature variation during filling. The isothermal RTM filling problem is a transient, free boundary problem of predicting the position of the resin flow front in the porous medium as a function of injection pressures and time. The resin is assumed to be nearly compressible and to display Newtonian behaviour. The fibre preform is assumed to be non-deforming. It is assumed that Darcy's law governs the relation between resin velocity, v, and pressure p, such that v = - p - KVp (1) where p is the viscosity and K is a tensor representing the permeability of the fibre preform. Preforms are usually constructed from several layers of fibre mat oriented in different directions. Permeabilities are experimentally calculated for mat samples and reported in terms of the principal directions of the mat. Thus, the average (through-thickness)permeability is a function of several factors, see for example Reference 4. Since permeabilities along the principal axes can easily differ by an order of magnitude, the ability to specify K on a local basis is essential in simulation. Let Q c R3 define the interior of the mold, r,,,the impermeable mold walls, r, the constant displacement injectors, and rgthe constant pressure injectors, so that the complete assembly includes sz = ourwurhurg (2) Let Q ( t ) E R denote the filled portion of the mold interior at time t and rs(t) the free surface at time t. On the air side of the surface, the capillary fringe is neglected and a constant pressure (e.g. atmospheric) is assumed in the unfilled portion of the mold {Q\n(t)}. The isothermal RTM filling problem (see Figure 1) is to find for any t > 0, rs(t): fl H R3and p:Q(t) H R such that V-(p-'KVp) = 0 in Q(t) (3) n-(p-'KVp) = 0 on r, n-(p-'KVp) = h(x) on r,, n.(p-lKVp) = - n.-dTS dt (4) (5) ISOTHERMAL RESIN TRANSFER MOLD FILLING 1407 Figure 1. Two-dimensional RTM mold. Resin flow front is a free surface where n denotes the vector normal to r.The quantityf= n * vis defined as the flux normal to the boundary. The mold filling problem is analogous to the Stefan problem, a class of free boundary problems used in modelling the melting of solids and crystallization of FILLING ALGORITHM The mold filling problem in equations (3)-(8) may be solved with a variety of numerical schemes, including fully implicit methods which solve simultaneouslyfor free surface location and pressure, as well as more conventional semi-implicitmethods which solve for pressure implicitly and satisfy the free surface condition (8) by an explicit method. We follow the latter approach, suggested by many researcher^,'^'-^ using a finite element solution to obtain pressures at discrete values of t followed by an explicit control volume scheme for updating the position of the free surface. The control volume scheme involves domain discretization into discrete subvolumes, where each such control volume contains one node of the finite element mesh. Fluid flux across control volume boundaries is calculated from the pressure solution. Net inflow to a control volume is tracked as the 'fill fraction'. When the volume is filled, the node contained in the volume is considered part of the next pressure solution, as summarized below. 1. Find FEM pressure solution: At the beginning of a new time step, the pressure field is calculated over the filled control volumes. 2. Calculate volume j u x : Darcy velocity and flux at the control volume boundaries are computed from the pressures calculated in step 1. 3. Locate the free surjihce: The time step is calculated as the minimum At required to fill a control volume using the flux calculated in step 2. The filled volume becomes part of the pressure field, moving the free surface to a new position. Finite element pressure solution At each time step, a free surface location r&)is given from the previous step. The problem of solving equation (3) subject to (4)-(7) is analogous to the classical steady-state heat conduction problem, which has the following weak formulation. Define the trial function and weight function spaces, u ={PIP V E H',Plr.ct, = 0,PIr, = ={W~E W H', wlr,"r, = 0) &)I (9) (10) 1408 R. S. MAIER ET AL. Given g, h, find p E U such that for all w E V , The Galerkin formulation (in two spatial dimensions) is based on a triangulation of the mold into nel elements, 12 % T = u i T i , i = 1, . . . , nel where the Ti are closed triangles with nodes (vertices) xi = (xi, yj), j = 1, . . . ,n (see Figure 2). We have chosen to work in the space of piecewise linear functions. Let p be the finite dimensional approximation to p, such that p" E U is a polynomial of degree one over each triangle. The vector p will denote the nodal values of p", i.e. and p"(x)= C1=lNi(x)pi,where the shape functions Ni(xj)= dij, i , j linear. The Galerkin formulation is then = 1, . . . ,n, are piecewise The elements of the n x n pressure stiffness matrix A are defined as VNi-(p-'KVNj)dR, i,j = 1,. . . ,n and the forcing vector b as bi = jrh NihdT,,, i = 1, . . . ,n In matrix notation, Ap = b (14) and the approximate pressure solution is obtained by solving a linear system of n equations in n unknowns. Control volume flux calculation The flux calculation approximates fluid velocities by the piecewise linear polynomials described in the previous section, n p-'KVNi(~)pi V(X) = i= 1 We use a node-centred control volume discretization to calculate flux and fluid volume fractions. The control volume discretization is built on the triangulation T (see Figure 2) and forms a set of closed subvolumes Ci, si FZ C = ujCi, i = I , . . . , n ISOTHERMAL RESIN TRANSFER MOLD FILLING 1409 Empty CV ...... ..... ........ ....... ....... ....... ........ ........ ....... ....... ....... .......... f) - Partially filled CV Filled CV & ...... ..... ....... ....... ........ ....... ....... ....... ........ ........ ....... ....... ..... ............... ............. .::.:::.::..:: .i;xs!;i;iiii: "..." ....... ......... ......... .... Effective free surface (P = 0) Flux Boundary :=::1fl::::::. .I Figure 2. Triangulation and control volume discretization of Q such that subvolume Ci contains vertex xi and no other node. Denoting Bi as the boundary of Ci, the flow rate into Ci at time t is where n is the unit normal to Bi. We define Bi as the set of line segments connecting element centroids with edge midpoints, as follows (see Figure 3). Associated with Bi is the set of elements Ei = { TjlxiE T j } .Without loss of generality, denote the vertices of Tj as xi, x i + l ,xi+z. Define the centroid of Ti as cj = iC:'=:xk 1 + xi+2).The segments of Bi in Ti are and the edge midpoints, mjl = ;(xi + xi+ 1) and mjz = 2(xi denoted by (cj, mil), (cj, mjz). Then qi can be written as an algebraic sum, ~~ (ljlnjl qi = Tj=Ei + IjZnjZ) 3 pLIKVNkPk (16) k= 1 where nil is the unit normal vector in the plane of Ti orthogonal to (cj,mjl), and Ijl = 1) cj - mil )I is the segment length. The coefficients of p in equation (16) are constant for all t and are assembled prior to the filling algorithm. Free surface location A node xi is included in the filled domain Q(t)if control volume Ci has a fill fraction of unity. Let Si(t) denote the fill fraction of Ci at time t, 1410 R. S. MAIER ET AL Figure 3. Control volume discretization.(a) The set Eiof elements supportedby node i, (b) centroid and edge midpoints for TI,(c) control volume Ciand boundary Bi,(d) superimposed FEM and control volume discretizations where lCil denotes volume adjusted for the porosity of the preform. At each time step, the fill fraction is updated explicitly. If qi(t) is the flow rate into C i at time t, then According to equation (7), the free surface location satisfies the relation p l r , = 0. We define the free surface location by the nodes in unfilled or partially filled volumes adjacent to filled nodes, i.e. xiis on the free surface if (a) Sj < 1,and (b) xi is adjacent to a node xi such that Si= 1. Observe in Figure 2 that the free surface intersects partially filled control volumes and that control volume flux is not actually calculated at the free surface. To address this fundamental discrepancy, some researchers have developed local refinement schemes in the flow front vicinity, e.g. Reference 10. Such schemes improve the local accuracy of the flow front approximation. However, we believe that if high accuracy in flow front calculations is needed, then an alternative filling algorithm satisfying more rigorous mathematical convergence criteria should be considered rather than local mesh refinement. Implementation Properties of the pressure stifiess matrix. The pressure stiffness matrix A in equation (14) has several important properties which lead to an efficientimplementation of the filling algorithm. The first property is sparsity, due to the structure of the finite element mesh. The order of A is ISOTHERMAL RESIN TRANSFER MOLD FILLING 1411 equal to the number of nodes, n, in the mesh. The number of non-zero entries in A is equal to the number of edges connecting adjacent nodes. Since the nodes of a finite element mesh typically are connected to only a few other nodes, the number of non-zeroes is far less than n2, usually a small multiple of n. The second and third properties of A are symmetry, A = AT, and positioe-definiteness, A(A) > 0. To demonstrate positive-definiteness,it is necessary to show that K is always positive-definite. Experimentalpermeability measurements are reported for principal mat directions as a diagonal matrix with strictly positive entries, D = diag(kll, kzz, k33).The tensor K is obtained by transforming from the principal directions of the mat to the Cartesian frame (or to local element co-ordinates),i.e. K = CDCT,where C is a rank-3, orthogonal rotation matrix which projects the principal axes of the mat into the Cartesian or local co-ordinate system. Since pre- or postmultiplication by an orthogonal matrix preserves the spectrum of an operator, I ( K ) = A(D) > 0. Given I ( K ) > 0, symmetry and positive-definitenessof A is a standard result in the finite element literature; see, for example, Reference 11. Since A is symmetric and positive-definite,it has a Cholesky factorization, LL’ = A, where L is a lower triangular matrix. It is also true that every submatrix of A inherits these two properties. Thus, if A is partitioned as then the matrix M has a Cholesky factorization M = LML: and .=(:; p) where LMw= u and t = (s - wTw)l’’. As a result, the Cholesky factor of the stiffness matrix can be computed row by row. This is exactly the property required for an efficient isothermal filling algorithm. Updating the pressure solution. Each time step At is calculated to fill one control volume. Filled volumes are considered part of the fluid phase and so the corresponding node becomes part of the fluid pressure calculation. The addition of a node to the pressure calculation corresponds to adding a single row and column to the stiffness matrix. The Cholesky factorization of the updated stiffness matrix can be updated directly, as in equation (20). The advantage is that the stiffness matrix A need only be factored one time, rather than reassembling and factorizing at every time step. The stiffness matrix A is assembled and stored prior to filling. The full matrix is stored in an adjacency structure. The adjacency structure consists of n adjacency lists and corresponding non-zero coefficients. The ith adjacency list includes the indices of nodes which are adjacent to (share an edge with) node xi. During the filling algorithm, nodes are added to the pressure field as control volumes are filled. Rows of A corresponding to these nodes are added to the Cholesky factor L using equation (20). Note that these rows must be permuted to reflect the node ordering imposed by the filling sequence. The data structure used to store L is an envelope structure. For each row of the matrix, all entries from the first non-zero up to the diagonal are stored. The envelope storage scheme is standard data structure for sparse matrix factorization. This choice permits the use of existing numerical software” for updating the Cholesky factorization and computing intermediate pressure solutions at each time step, with only minor modifications. 1412 R. S. MAIER ET AL. In practice, the algorithm will often fill more than one node in a single time step, despite the fact that the time step is calculated to fill only one volume. This occurs most typically in regular discretizations because a tolerance is used to define the fill fraction constituting a ‘filled’ control volume (e.g. 99 per cent). C V F E algorithm. The CVFE algorithm requires an extensive set of inputs and initialization steps. For the case of a two-dimensional thin shell geometry in three-dimensional space, these initialization steps include: specification of a triangulation T, specification of a control volume discretization C, specification of local permeabilities and element thickness, rotation of permeabilities to local element co-ordinates, calculation of adjacency data structure for A, assembly of A in adjacency structure, assembly of flow rate coefficient matrix. The iterative part of the algorithm computes the filling sequence, using the integer arrays perm and invp to denote the ordering of A (the filling sequence) used in the Cholesky factorization. The notation perm(i) = k means the original node k is the ith node in the new ordering. The element invp(k) gives the position in perm where the node originally numbered k resides, i.e. perm(invp(k)) = k. We use the array subscript notation bi = b(i) interchangeably. t = 0; 1 = 0; m = 0; filled = false; while (not filled) compute forcing vector b {add row(s) to pressure stiffness factor L } {add filled control volumes to ! 2 ( t ) } for i = 1 , . . . , n if Si(t) = 1 and xi3 n(t), {increment number of filled volumes} m=m+l; perm(i) = m; invp(m) = i; {scatter row i from adjacency structure of A to full vector} w ( j ) + a i j , j = l , . . . , n; {gather permuted row i into envelope structure for L} Lij t w(invp(j)), j = 1, . . . ,n; end if end for {solve updated pressure system} b(perm(i)) t b(i), i = 1, . . . , n; {permute forcing vector} update Lij,i = I + 1, . . . , m , j = 1, . . . ,m {equation (20)) solve y c Ly = b solve p c LTp = y; 1 = m; {updated dimension of L } p(invp(i)) t pi, i = 1, . , . ,rn; {restore solution to original order) (update fill fractions} ISOTHERMAL RESIN TRANSFER MOLD FILLING 1413 compute qi(t),i = 1, . . . ,n; if qi(t) = 0, i = 1, . . . ,n, STOP; {mold cannot be filled} At = mini[(l - Si(t)) lCil/qi(t)],i = 1, . . . , n; Si(t At) = &(t) + At&), i = 1, . . . ,n; t = t + At; if S i ( t ) = 1, i = 1, . . . ,n, filled = true; + end while The order in which control volumes are filled determines the ordering of A during the Cholesky factorization. A more efficient ordering could be obtained by using a symbolic factorization algorithm, such as reverse Cuthill-McKee' to find an ordering which reduces the maximum envelope band-width. Such a procedure reduces the number of non-zero elements in L and hence the computational effort in solving L y = b and LTx = y . This possibility will be addressed in the context of further research on the application of direct factorization methods for large-scale RTM simulation and parallel computation. Computational complexity This section analyses the computational requirements of the filling algorithm as a function of the problem size. The analysis is based on several assumptions about typical models and is not a worst-case analysis of complexity. The CVFE algorithm requires O(n)iterations or time steps, one per control volume (in practice, more than one volume may fill per time step). Each iteration requires the four procedures as summarized below. for k = 1, . . . , n compute forcing vector b add row(s) to L solve updated pressure system update fill fractions end while O(n) operations O(n) operations O(/C"~)operations O(n) operations Three procedures require O(n) operations per iteration, or O(n2)operations for all iterations. One procedure, solving the updated pressure system, requires O(k"5) operations per iteration, where k is the iteration number. This procedure dominates the total computation and is explained below. The updated pressure system requires several sparse-matrix back-substitutions using L. The number of operations in a back-substitution is proportional to the number of non-zeroes in L. It is assumed that the A originally has O(n) non-zeroes. This is reasonable since the maximum adjacency list length is typically a small constant (e.g. 6). However, it is also assumed that A has the structure of an n x n Laplacian matrix, with a bandwidth of O(&), and that no reordering scheme is used. Then the fill-in of L is O(n1'5)non-zeroes, corresponding to fill-in between the per iteration as rows are added to L. bands. It is assumed that fill-in occurs at the rate O(IC"~) Using the following relationship, k'.5 < k= 1 & k k= 1 = $&(n' + n) 1414 R. S. MAIER ET AL. we bound the total computational effort as O(n2”).Thus, the complete CVFE algorithm requires operations. A CVFE algorithm which assembles and factors the stiffness matrix at each iteration would theoretically require O(n2) operations per time step and O(n3) in total. The introduction of reordering algorithms could further reduce the complexity of both the CVFE algorithm described in this paper as well as conventional approaches. NUMERICAL RESULTS This section summarizes implementation and performance details of the filling algorithm. The details include type of architecture and source language, method of validation, comparison with related codes, and timing results for several test problems. The filling algorithm has been implemented in Fortran 77 for the Silicon Graphics (SGI) workstation architecture and given the code name ISOFIL. ISOFIL was developed under a systems integration plan based on the SGI Explorer program and makes use of extensions to Fortran 77, including the Fortran POINTER data type and the malloc procedure call. ISOFIL also includes routines from two public domain software libraries, BLAS (level 1)14and SPARSPAK.12 All performance results reported in this section are based on the SGI model 4D-35 workstation. Numerical validation of ISOFIL so far has included evaluation of mass balance. In one validation exercise, a 10 cm radius, centre-gated, disk mold was discretized with 800 triangles and injected at the constant flow rate of 1 cm3 assuming a void fraction of 70 per cent, anisotropic permeability (k, = 1, kz2 = 0.3) and two fibre orientations. The simulated filling time was 213.8 s compared to the expected (analytical) 219.6 s, or about 3 per cent relative error. The same model was evaluated using a constant pressure injection of 1 kg/cm2. The mass influx was approximated by the flux across the control volume boundaries surrounding the injector. The resulting approximation was 214.1 cm3 to fill the mold, versus the expected (analytical) 219.6 cm3. The CPU time was 5 s, including input and output. A qualitative evaluation of the simulated flow fronts indicates that flow front shape is determined by element shape. This result can also be inferred from an inspection of Figure 2. Highly elongated elements lead to elongated control volumes. Elongated volumes may fill before neighbouring volumes begin to fill, in a locally non-physical manner. This effect demonstrates the need for a relatively uniform mesh with a good aspect ratio for the triangles. The performance of ISOFIL was compared to a predecessor code, LIMS, from the University of Delaware.” ISOFIL uses the same CVFE approach as LIMS to model pressure and fluid velocity. There are minor differences in how control volume flux is calculated. The primary differences are that LIMS assembles and factors the pressure stiffness matrix and the flux stiffness matrix at each time step of the CVFE algorithm. As a result, the performance differential between the two codes increases with n, the number of nodes. For a 2213-node, 4443-triangle model of the Ford Aerostar Crossmember (see below), the CPU times were 230 s for ISOFIL and 22 389 s for LIMS 2.2, a speedup factor of approximately 100. A set of four test problems are presented in Figure 4, including a plaque, disk, auto crossmember and aircraft keel prototype. The plaque and disk models are simple two-dimensional geometries, while the crossmember and prototype keel box are thin-shell, three-dimensional structures. These models have been simulated under various conditions, including different choices of injector/vent locations, material type (permeability and fibre orientation). The performance results are presented in Table I. The larger test problems require several minutes of CPU ISOTHERMAL RESIN TRANSFER MOLD FILLING 1415 Figure 4. Four problems with flow front histories. Clockwise from upper left: disk, crossmember, keel prototype, plaque time. The time to read the input deck (element mesh and material properties) is included in the results; however, it is not a major fraction of the total time. The error in mass balance ranges up to 3 per cent for the test problems and is calculated as described above for the constant pressure injection case. 1416 R. S. MAIER ET AL. Table I. ISOFIL performance on four models. Results were obtained on an SGI 4D-35, CPU time includes I/O. Speedup is the ratio of LIMS 2.2 CPU time to ISOFIL CPU time Problem Disk Plaque Xmbr Proto Nodes Elements Sec. 442 925 2213 2066 800 1728 4443 4116 22 230 188 Mass bal. (%) Speedup 2.60 0.02 0.45 0-39 23 33 97 5 na CONCLUSIONS The isothermal RTM filling algorithm has a computational complexity of O(n2”), compared to more general RTM algorithms which also employ the CVFE formulation but require O(n3) computation. This relative advantage results in a 100-fold performance improvement over a similar code for a 2213-node model, while obtaining the same solution accuracy. The speed of the filling simulation is critical to applying simulation results to actual mold design. A fast and flexible simulation tool allows engineers to include modelling in the design process. The ISOFIL code is currently being used for interactive filling simulation of structural aircraft components in connection with Army procurement projects. The complete software system permits interactive graphical manipulation of mesh and material properties, as well as the location and specification of injection pressure/displacement time profiles. The details of this complete system will be published in a future paper. Interactive simulation (and real-time control) is now feasible for small (n x 1000)problems on high performance workstations and supercomputers. However, the computational requirement of O(n2’5) operations still prohibits interactive simulation of refined three-dimensional models involving n > 10’ nodes (massively parallel supercomputers are capable of about 10” floating point operations per second). We are interested in simulations which require a matter of seconds, or at most a few minutes, of real time. This motivates the need for further investigation of filling algorithms which depart from the conventional CVFE strategy. ACKNOWLEDGEMENTS We acknowledge the advice and assistance of Mathematician David J. Eyre, at the Army High Performance Computing Research Center, University of Minnesota. REFERENCES 1. V. R. Voller and Y. F. Chen, ‘Prediction of filling times of porous cavities’, Inr. j. numer. methodsjuids, in press. 2. K. Meissner and P. Sincebaugh,‘Preventing mechanical failures in resin transfer molding using embedded sensors and neural networks’, Preprint, US.Army Research Laboratory, Materials Directorate, Watertown, MA 02172-0001. 3. C. L. Tucker and R. B. Dessenberger, ‘Governing equations for flow through stationary fiber beds’, in S. G. Advani (ed.),Flow and Rheology in Polymer Composites Manufacturing, Elsevier, Amsterdam, 1994. 4. S. Advani, M. V. Bruschke and R. S. Parnas, ‘Resin transfer molding’,in S. G. Advani (ed.), Flow and Rheology in Polymer Composites Manufacturing, Elsevier, Amsterdam, 1994. 5. A. Friedman, Partial Diferential Equations of Parabolic Type, Prentice-Hall, Englewood Cliffs, N.J.,1964. 6. J. Crank, Free and Moving Boundary Problems, Oxford University Press, Oxford, 1984. 7. H. P. Wang and H. S. Lee, ‘Numerical techniques for free and moving boundary problems’, in C. L. Tucker 111(ed.), Fundamentals of Computer Modeling for Polymer Processing, Hanser, Munich, 1989. ISOTHERMAL RESIN TRANSFER MOLD FILLING 1417 8. W. 9. Young, K.Han, L. H. Fong, L. J. Lee and M. J. Liou, ‘Flow simulation in molds with preplaced fiber mats’, Polymer Composites, 12, 391 (1991). 9. S. Advani and M. Bruschke, ‘A finite element/control volume approach to mold filling in anisotropic porous media’, Polymer Composites, 11, 398405 (1990). 10. W. B. Young, L. J. Lee and M. J. Liou, ‘Modification of control volume finite element method in mold filling simulation’, Report No. ERCINSM-P-91,NSF Engineering Research Center for Net Shape Manufacturing, The Ohio State University, Columbus, OH 43210, January 1991. 11. T. J. Hughes, The Finite Element Method: Linear Static and Dynamic Finite Element Analysis, Prentice-Hall, Englewood Cliffs, N.J., 1987. 12. SPARSPAK, netlib@ornl.gov. 13. A. George and J. Liu, Computer Solution of Large Sparse Positive Definite Systems, Prentice-Hall, Englewood Cliffs, N.J., 1981. 14. Basic Linear Algebra Subroutines, netlib@ornl.gov. 15. S. Advani and M. Bruschke, Liquid Injection Molding Simulation User’s Manual Version 2.0, Center for Composite Materials, University of Delaware, Newark, DE 19716, December 1992.

1/--страниц